Uploaded by Rosemarie Villanueva

# 01introductiontomechanicalmetallurgy-121105104349-phpapp02 ```Introduction to mechanical
metallurgy
Chapter 1
Subjects of interest
• Introduction to mechanical metallurgy
• Strength of materials – Basic assumptions
• Elastic and plastic behaviour
• Average stress and strain
• Tensile deformation of ductile metals
• Ductile vs brittle behaviour
• What constitute failure?
• Concept of stress and the types of stresses
• Units of stress and other quantities
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
Objectives
• This chapter provides a background of continuum
description of stress and strain and extends it to the defect
mechanisms of flow and fracture of metals.
• Elastic and plastic behaviours of metals are highlighted
and factors influencing failure in metals are finally
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
Introduction
Mechanical metallurgy : Response of metals to forces or loads.
Mechanical assessment of
Materials
• Structural materials
• Machine, aircraft, ship, car etc
We need to know
limiting values of which
materials in service can
withstand without
failure.
Suranaree University of Technology
Forming of metals into
useful shapes
• Forging, rolling, extrusion.
• drawing, machining, etc
We need to know conditions
of load and temperature to
minimise the forces that are
needed to deform metal
without failure.
Tapany Udomphol
May-Aug 2007
Strength of materials
Strength of materials deals with relationships between;
• internal resisting forces
• deformation
, which act on some part of a body (member) in equilibrium.
• In equilibrium condition, if there are the
external forces acting on the member,
there will be the internal forces resisting
the action of the external loads.
Internal force
External force
∫ σdA
P
• The internal resisting forces are usually expressed by the
stress acting over a certain area, so that the internal force is the
integral of the stress times the differential area over which it acts.
P = ∫ σdA
Suranaree University of Technology
Tapany Udomphol
…Eq.1
May-Aug 2007
Assumptions in strength of materials
The body (member) is
• Continuous:
No voids or empty spaces.
• Homogeneous: Has identical properties at all
points.
• Isotropic:
Has similar properties
in all directions or orientation.
Remark:
Anisotropic is when
the body has
property that varies
with orientation.
Macroscopic scale, engineering materials such
as steel, cast iron, aluminium seems to be
continuous, homogeneous and isotropic.
Microscopic scale, metals are made up of an
aggregate of crystal grains having different
properties in different crystallographic directions.
However, these crystal grains are very small,
and therefore the properties are homogenous
in the macroscopic scale.
Suranaree University of Technology
Tapany Udomphol
Microstructure of
low carbon steel
May-Aug 2007
Elastic and plastic behaviour
• All solid materials can be deformed
when subjected to external load.
stress
Elastic
limit
• In elastic region, stress is proportional to
strain. This follows Hook’s law up to the
elastic limit . The material now has elastic
behaviour.
• At the elastic limit, when the load is
removed, the material will change back to
its original shape.
Maximum
tensile strength
Fracture
σmax
Elastic Plastic
• Beyond the elastic limit, material
permanently deformed or the material has
undergone plastic deformation.
strain
Load and extension curve of
Note: elastic deformations in metals are relatively small
in comparison to plastic deformations.
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
Average stress and strain
Lo
Lo+ δ
Lo
P
• A uniform cylindrical bar which is
subjected to an axial tensile load P.
The original gauge length Lo has
undergone a slight increase in
length to Lo+ δ with a slight
decrease in diameter.
The external load P is balanced by
the internal resisting force, giving
the equilibrium equation;
• The average elastic strain e is
the ratio of change in length to the
original length.
If the stress σ is uniform over the area
A, σ = constant, then
…Eq.2
Internal
force
∫σdA
Suranaree University of Technology
P
P = ∫ σdA
P = σ ∫ dA = σA
δ
∆L L − Lo
=
=
e=
Lo Lo
Lo
External
force
The average stress σ =
Tapany Udomphol
P
A
…Eq.3
May-Aug 2007
Average stress and strain
• In general, the stress is not uniform over the area A
average stress.
• On a microscopic scale, metals consist of more
than one phase and therefore give rise to
nonuniformity of stress.
stress
• Below the elastic limit, Hook’s law
can be applied, so that the average
stress is proportional to the average
strain,
σ
=E
ε
…Eq.4
The constant E is the modulus of
elasticity or Young’s modulus.
Maximum
tensile strength
Elastic
limit
Fracture
σmax
strain
Load and extention curve of
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
Tensile deformation of ductile metal
• In tension test, specimen is subjected to axial tensile load
until fracture. Load and extension are measured and expressed
as stress and strain, see Fig.
• The initial linear portion of the curve (OA) is the elastic region,
following Hook’s law.
• Point A is the elastic limit (the greatest stress that the metal
can withstand without undergone permanent or plastic
deformation. A’ is the proportional limit where the curve
deviates from linearity.
D
Elastic
limit
A’
A
B
• The slope of the linear portion is the modulus of elasticity.
• Point B is the yield strength, defined as the stress which will
produce a small amount of strain equal to 0.002 (OC).
• As the plastic deformation
increases, the metal
becomes stronger (strain
hardening) until reaching the
ultimate tensile strength D.
• Beyond D, metal necks
(reduce in x-section). Load
needed to continue
deformation drops off till
failure.
Suranaree University of Technology
Tapany Udomphol
C
May-Aug 2007
• Brittle metals such as cast iron
show small amounts of plasticity
before failure.
• For engineering materials,
adequate ductility is important
because it allows the materials to
redistribute localised stresses.
stress
• Completely brittle materials i.e.,
ceramics would fracture almost at
the elastic limit.
stress
Ductile and brittle behaviour
strain
strain
Completely brittle
Slightly brittle with
small amount of
ductility
• Fracture behaviour of metal (ductile or brittle) also depends on
some conditions, i.e., temperature, tension or compression, state
of stresses, strain rate and embrittling agent.
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
What constitute fracture?
1) Excessive elastic deformation
2) Yielding or excessive plastic deformation
3) Fracture
Elastic
energy
Plastic
energy
strain
Good structural
components in
service without
failure
Nature of Materials
Structural design
Suranaree University of Technology
stress
Three general ways that cause failures in structural
members and machine elements:
Tapany Udomphol
May-Aug 2007
Excessive elastic deformation
1) Excessive elastic deformation under
condition of stable equilibrium.
EX: too much deflection in a shaft can cause
wear in bearing and damage other parts.
stress
• Failure due to excessive elastic deformation are controlled by
the modulus of elasticity not the strength of the materials.
Two general types of excessive elastic
deformation:
Elastic
energy
strain
2) Excessive elastic deformation under
condition of unstable equilibrium.
EX: A sudden deflection or buckling of a slender column.
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
Excessive plastic deformation
• Excessive plastic deformation occurs when the elastic
limit is exceeded yielding.
stress
• Yielding produce permanent change of shape and can
cause fracture.
EX: When component changed in shape,
it cannot function properly any longer.
Elastic
energy
• Failure by excessive plastic
deformation is controlled by the yield
strength of the materials. Even in more
is still a significant parameter.
Plastic
energy
strain
Large deformation that cause
failure in a pipe
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
Fracture
Metals fail by fracture in three general ways:
1) Sudden brittle fracture
Ex : some ductile metal such as plain carbon steel
will undergo ductile to brittle transition with
and triaxial state of stresses.
2) Fatigue, or progressive fracture
Most fracture in machine parts are due to fatigue
(subjected to alternating stresses). Failure is due
to localised tensile stress at spot or notch or stress
concentration.
3) Delayed fracture
Ex: Stress-rupture failure, which occurs when a
metal has been statistically loaded at an elevated
temperature.
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
Working stress
To prevent structural members or machine elements from failure,
such members should be used under a stress level that is lower than
its yield stress σo. This stress level is called the working stress σw.
According to American Society of Mechanical Engineering
(ASME), the working stress σw may be considered as either the
yield strength σo or the tensile strength σu divided by a number
called safety factor.
σw =
…Eq.5
Where σw
σo
σu
No
Nu
σo
No
or
σw =
σu
Nu
…Eq.6
= working stress
= yield strength
= tensile strength
= safety factor based on yield strength
= safety factor based on tensile strength
Safety factor depends on loading/service conditions, consequences, etc.
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
Concept of stress and the type of
stresses
Definition: stress is force per unit area.
There are two kinds of external forces which may act on a body;
1) Surface forces : forces distributed over the surface of the body,
i.e., hydrostatic pressure
2) Body forces : forces distributed over the volume of the body,
i.e., gravitational force, magnetic force, centrifugal force, thermal
stress.
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
Stress at a point
• Consider a body having forces F1…F4
acting on it, see Fig (a). The body is cut by a
plane passing through point O. If one half is
removed and replaced by an equivalent force
F, acting on the x-sectional area A to remain
the static equilibrium, see Fig (b).
• We can resolve F into component normal to
the plane Fn and tangential to the plane Fs.
(a) Equilibrium of
an arbitrary body.
• The concept of stress at a point is shrinking
the area A into infinitesimal dimensions.
…Eq.7
σ = lim
∆A→0
Fn
A
and
τ = lim
∆A→0
Fs
A
…Eq.8
Note: σ and τ depend on the orientation of the plane
passing through P and will vary from point to point.
Suranaree University of Technology
Tapany Udomphol
(b) Force acting
on parts.
May-Aug 2007
The total stress can be resolved into two components;
1) Normal stress σ perpendicular to A.
2) Shear stress τ lying in the plane of the area.
• The force F makes an angle θ with the normal z to the plane x-y of
the area A.
• The plane containing the normal z and F intersects the plane A along
a dash line that makes an angle φ with the y axis.
The normal stress
is given by
…Eq.9
σ=
F
cos θ
A
F
Resolutions of total stress into its
components.
Suranaree University of Technology
The shear stress in the plane
acting along OC has the
magnitude.
F
τ = sin θ
A
…Eq.10
x direction τ =
F
sin θ sin φ …Eq.11
A
y direction τ =
F
sin θ cos φ …Eq.12
A
Tapany Udomphol
May-Aug 2007
Concept of strain and types of
strain
The average linear strain was defined as the ratio of the
change in length to the original length.
δ
∆L L − Lo
e=
=
=
Lo Lo
Lo
Where e = average linear strain
δ = deformation.
…Eq.2
Strain at a point is the ratio of the deformation to the gauge
length as the gauge length 0.
True strain or natural strain is the strain as the change in
linear dimension divided by the instantaneous value of the
dimension.
Lf
Lf
dL
ε=∫
= ln
…Eq.13
L
L
o
Lo
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
Shear strain
• Shear strain is the angular change in a right angle.
• The angle at A, which is originally 90o, is decreased by
a small amount θ when the shear stress is applied.
• The shear strain γ will be given by
a
θ
h
a
γ = = tan θ = θ
h
…Eq.14
A
Shear strain
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
Units of stress and other quantities
• Following SI unit
Length
metre (m)
Mass
kilogram (kg)
Frequency
(s-1, Hz)
Time
second (s)
Force
Newton (N)
Electric current
ampere (A)
Stress
(N.m-2, Pa)
Temperature
Kelvin (K)
Strain
dimensionless
Amount of substance
mole (mol)
Luminous intensity
candela (cd)
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
Example: The shear stress required to nucleate a grain boundary
crack in high-temperature deformation has been estimated to be
 3πγ b G 

τ = 
 8(1 − ν ) L 
1
2
Where γb is the grain boundary surface energy ~ 2 J.m-2, G is shear
modulus, 75 GPa, L is the grain boundary sliding distance, assume =
grain diameter 0.01 mm, and the Poisson’s ratio ν = 0.3.
Checking the unit
1
2
1
 Nm N 
1
9
 3π × 2 × 75 × 10
2
 2 × 2
2 2
7
−2
N 


N
=
=
15
.
89
×
10
N
.
m
τ
m
m
−2
−3 
 =
 = 2
τ =
 8(1 − 0.3) × 10 × 10 
4 


m

m 
m



τ
= 158.9 MN .m −2 = 158.9 MPa


Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
References
• Dieter, G.E., Mechanical metallurgy, 1988, SI metric edition,
McGraw-Hill, ISBN 0-07-100406-8.
• Sanford, R.J., Principles of fracture mechanics, 2003,
Prentice Hall, ISBN 0-13-192992-1.
• www.indiamart.com.
• www.technion.ac.il/.../ Figures/Light-steel.jpg
• www.uvi.edu
Suranaree University of Technology
Tapany Udomphol
May-Aug 2007
```